University of Wisconsin Milwaukee
UWM Digital CommonsTheses and Dissertations
Coking Resistance of Alumina Forming Cast
Austenitic Stainless Steels
Lizeth Nayibe Ortiz Reyes University of Wisconsin-Milwaukee
Follow this and additional works at:https://dc.uwm.edu/etd Part of theMaterials Science and Engineering Commons
This Thesis is brought to you for free and open access by UWM Digital Commons. It has been accepted for inclusion in Theses and Dissertations by an authorized administrator of UWM Digital Commons. For more information, please firstname.lastname@example.org.
Ortiz Reyes, Lizeth Nayibe, "Coking Resistance of Alumina Forming Cast Austenitic Stainless Steels" (2017). Theses and Dissertations. 1520.
COKING RESISTANCE OF ALUMINA FORMING CAST AUSTENITIC STAINLESS
Lizeth Nayibe Ortiz Reyes
A Thesis Submitted in
Partial Fulfillment of the
Requirements for the Degree of
Master of Science
The University of Wisconsin-Milwaukee
COKING RESISTANCE OF ALUMINA FORMING CAST AUSTENITIC STAINLESS STEELS
Lizeth Nayibe Ortiz Reyes
The University of Wisconsin-Milwaukee, 2017 Under the Supervision of Dr. Benjamin C. Church
Coking is the process of carbon deposition from a gas phase that is encountered in
many reforming, cracking and other high temperature processes. Coking in certain
petrochemical processes can lead to carbon build up causing reduced process
efficiency, corrosive attack, and degradation of the alloy. Steam cracking of
hydrocarbons is one of the most important process for manufacturing many base
chemicals such as ethene, propene and other. A major influence on the energy
efficiency and economics is the formation of coke on the inner wall of the reactors. With
the accumulation of coke on the walls, eventually metallurgic constraints of the reactor
material will force to stop the process and de-coke the reactors resulting in loss of
efficiency with negative effect on the economics of the process.
Materials used in these processes are fabricated from HP alloys that rely on the
formation of a chromium oxide (chromia) layer as a protective layer between the bulk
material and chemical byproducts. However, strong oxidation, carburization, sulfidation
or nitriding can occur if the environment does not promote chromium oxide formation or
More recent alloys that form an alumina-based oxide layer have been recently
developed for structural use in aggressive oxidizing environments. These alloys,
commonly known as AFA alloys, form a protective layer of aluminum oxide (alumina)
showing a promising combination of oxidation resistance, creep resistance, tensile
properties, and potential for good welding behavior.
An experimental high temperature coking atmosphere was constructed and used to
evaluate the effects of temperature, time and metal surface roughness on the carbon
deposition of two alumina forming alloys (2.6% and 3.7% Al content each). Coking
conditions were simulated with multiple atmospheres including CO-H2 mixtures at
moderate temperatures and ethane at higher temperatures. Carbon deposition was
tracked using specific mass change of the samples as a function of exposure times and
conditions. Results obtained with the alumina forming alloys were compared to a
baseline HP alloy. The materials were analyzed using XRD, SEM, and optical
microscopy to characterize the oxide layer formation, carbon deposition layers and
carbon attack, and changes to base metal microstructure. Raman spectroscopy was
used to characterize the carbon deposits.
The overall resistance of the alumina-forming alloys relative to the traditional chromia
forming alloys is described. Overall, AFA alloys showed better coking resistance to
more aggressive environments that involve high temperature and longer times of
exposure than traditional chromia-forming alloy. Therefore, this particular coking
resistance make AFA alloys suitable for a wide range of energy production, chemical
and process industry applications, resulting in significant cost and energy savings as
© Copyright by Lizeth Ortiz, 2017 All Rights Reserved
My loving parents,
Jorge and Mabel
whose words of encouragement and support
TABLE OF CONTENTS
LIST OF FIGURES ...ix
LIST OF TABLES ... xiv
LIST OF ABBREVIATIONS ...xv ACKNOWLEDGMENTS ... xvi CHAPTER 1. INTRODUCTION... 1 1.1. Background ... 2 1.2. Literature review ... 4 1.2.1. Current materials ... 4 1.2.2. AFA Alloys ... 4 1.2.3. Al2O3 vs. Cr2O3 ... 8
1.2.4. Crystal structure of AFA alloys ... 10
1.2.5. Oxidation ... 11 1.2.6. Coking ... 18 1.2.7. Cyclic conditions ... 29 CHAPTER 2. METHODOLOGY ... 31 2.1. Material Composition ... 31 2.2. Sample preparation ... 32
2.2.1. Influence of surface roughness ... 34
2.2.3. Cyclic conditions ... 36
2.3. Pre-Oxidation test ... 36
2.4. Coking test ... 38
2.4.1. Influence of surface roughness and atmosphere ... 39
2.4.2. Influence of time and temperature under C2H6 atmosphere ... 40
2.5. Cyclic conditions ... 41
2.6. Characterization ... 42
2.6.1. Change in mass ... 42
2.6.2. Scanning Electron Microscopy (SEM) ... 43
2.6.3. Energy Dispersive Spectroscopy (EDS) ... 43
2.6.4. Raman Spectroscopy ... 43
CHAPTER 3. RESULTS ... 45
3.1. Influence of surface roughness and gas atmosphere ... 45
3.1.1. Carbon deposition in CO-H2-H2O atmosphere... 46
3.1.2. Carbon deposition in C2H6/Ar atmosphere ... 49
3.1.3. Summary ... 56
3.2. Influence of time and temperature under C2H6 atmosphere ... 57
3.2.1. Pre-oxidation treatment ... 57
3.2.2. Influence of time and temperature ... 59
3.3. Cyclic conditions ... 65
3.3.1. Summary ... 69
CHAPTER 4. ANALYSIS AND DISCUSSION ... 70
4.1. Influence of surface roughness and gas atmosphere ... 70
4.2. Influence of time and temperature under C2H6 atmosphere ... 72
4.2.1. Pre-oxidation in Steam ... 72
4.2.2. Influence of time and temperature ... 73
4.3. Cyclic conditions ... 74
CONCLUSIONS ... 75
FUTURE WORK... 78
REFERENCES ... 79
APPENDIX A – DIMENSIONS OF SAMPLES ... 85
Influence of surface roughness ... 85
Influence of time and temperature under C2H6 atmosphere ... 86
Cyclic conditions ... 87
APPENDIX B – SEM OF INFLUENCE OF SURFACE ROUGHNESS ... 88
Carbon deposition in CO-H2-H2O atmosphere ... 88
Carbon deposition in C2H6 atmosphere ... 89
LIST OF FIGURES
Figure 1. Phase diagram of Fe-Cr-Al-(20, 25, 30) Ni-1Nb-2Mo-0.1C showing limitations
of Cr and al additions in a range of 600 to 1200 °C (right); and at 650, 700, 750 and
800°C phases, predicted by thermodynamic calculation. ... 6
Figure 2. Superimposed ternary phase diagram of Fe-Cr-Ni near the Fe-rich corner at
1200 °C (bold lines) and at 800 °C (broken lines). Arrows indicate the direction of phase
boundaries shifting by the Al addition due to the strong δ-Fe stabilizing effect of Al relative to γ-Fe.2 ... 6 Figure 3. A schematic representation of (a) growth rate data and (b) thermodynamic
stability data for specific oxides. ... 10
Figure 4. BSE BSE-SEM image from CAFA7 (left) and HP (right) alloy tested at 800°C
in air for 2000 hours. ... 13
Figure 5. BSE-SEM of AFA 4-1 (4Al/0.6Nb/0.1ti) after 100h at 900 °C in air. ... 14
Figure 6. Ellingham/Richardson diagram for metal oxides. Standard free energies of
formation in function of Temperature... 15
Figure 7. Free energy changes, ΔG, expressed as oxygen potential for various oxidation reaction temperatures. ... 16
Figure 8. Mass change of samples during steam pre-oxidation treatments at 915 °C. . 18
Figure 9. Schematic diagram of the heterogeneous catalytic mechanisms for coke
deposition. ... 23
Figure 11. Schematic depth profile illustrating a suggested mode of formation of
nanoparticles of Ni that can act as potential catalytic agents for producing carbon
filaments. ... 29
Figure 12. Notation for dimensions of samples after cutting ... 33
Figure 13. Some of the samples used for tests. ... 33
Figure 14. Oxidation Apparatus ... 37
Figure 15. Thermal pre-oxidation under 100 % steam used to prepare samples prior to coking tests. ... 38
Figure 16. Scheme of the coking furnace used. ... 38
Figure 17. Furnace used to carry out the coking experiment. ... 39
Figure 18: Coking profile temperature carried out. The time at the peak temperature (600 °C) was 169 h with CO/CO2 atmosphere; for C2H6 atmosphere the time at the peak temperature (850 °C) was 100 h. ... 40
Figure 19. Design of experiments for the evaluation of temperature and time under C2H6 gas atmosphere ... 41
Figure 20. Experimental procedure carried out for cyclic conditions ... 42
Figure 21. Samples prior to coking test of CO-CO2-H2O atmosphere ... 46
Figure 22. Mass difference per surface area of samples after exposure to CO/H2 for 169h at 600°C. ... 47
Figure 23. Samples after coking with CO CO-CO2-H2O at 600 °C for 169 h. ... 48
Figure 24. Photo of the crucible with samples after coking with CO CO-CO2-H2O at 600 °C for 169 h ... 48
Figure 25.SEM Images at 2000x of the surface after exposition to CO/CO2 atmosphere
at 600°C for 169 hours. ... 49
Figure 26: SEM cross-sections images at 5000x of samples after exposition to CO/CO2
atmosphere at 600°C for 169 hours. ... 49
Figure 27. Carbon deposited during C2H6 atmosphere at 850 C for 100 hours ... 50
Figure 28. Photo of the crucible with some of the samples after coking with C2H6 at 850
C for 100 hours. ... 50
Figure 29. Samples after coking with C2H6 at 850 C for 100 hours. ... 51
Figure 30. Results of Raman Spectroscopy performed on the carbon deposits. ... 52
Figure 31. Mass difference per surface area of samples after exposure to C2H6 for
100h at 850 °C. ... 52
Figure 32: SEM images of the surface of samples after exposure to C2H6/Ar atmosphere
at 850 °C for 100 hours. ... 53
Figure 33. SEM image of the surface at 3000x of 3.7%Al alloy with EDS results. ... 54
Figure 34: SEM cross-sections of samples after exposure to C2H6/Ar atmosphere at 850
°C for 100 hours. ... 54
Figure 35. EDS linescan of cross section of HP-Nb alloy exposed to C2H6/Ar
atmosphere at 850 °C for 100 hours. ... 55
Figure 36. EDS linescan of cross section of 3.7%Al and 2.6%Al AFA alloys exposed to
C2H6/Ar atmosphere at 850 °C for 100 hours. ... 56
Figure 37. Samples after pre-oxidation treatment ... 57
Figure 39. Change in mass of samples after exposure to C2H6 for 1, 6 and 24 hours at
850, 950 and 1050 °C at each temperature. ... 60
Figure 40. Change in mass of samples after exposition to C2H6 for 1, 6 and 24 hours at 850, 950 and 1050 °C. ... 60
Figure 41. Samples after exposure to C2H6 for 24 h at 850 °C. ... 61
Figure 42. SEM cross section of samples after exposure to C2H6 at 850 °C ... 62
Figure 43. SEM cross section of samples after exposure to C2H6 at 950 °C ... 63
Figure 44. SEM cross section of samples after exposure to C2H6 at 1050 °C ... 64
Figure 45. EDS of cross section of alloys exposed to C2H6 atmosphere at 1050 °C for 6 hours. ... 64
Figure 46. Mass change for each step of one cycle coking/de-coking ... 66
Figure 47. SEM cross-sections at 5000x magnification. a) Pre-oxidation with 100% steam for 12 h at 850°C and 1 h at 915°C; b) coking with 25%C2H6/75%Ar for 6 h at 1050°C; c) de-coking with air for 15 min at 1050°C; d) de-coking with 100% steam for 1 h at 915°C ... 68
Figure 48. Comparison of effect of atmosphere on cross sections of samples ... 71
Figure 49. SEM of surface and cross section for samples ground to 1200-grit and exposed to CO-CO2-H2O at 600 C for 169 hours. ... 88
Figure 50. SEM of surface for samples ground to 1200-grit and exposed to C2H6-Ar at 850°C for 100 hours. ... 89
Figure 51. SEM cross section from surface (left) to base metal (right) of 2.6% Al exposed to C2H6 at 1050 °C for 24 hours. ... 90
Figure 53. SEM cross section of samples after exposure to C2H6 for 1 hour ... 92
LIST OF TABLES
Table 1. Comparison of Al2O3 vs Cr2O3 oxide scales ... 9
Table 2. Nominal compositions of the alloy samples. ... 32
Table 3. Surface roughness average for each grit sandpaper used. ... 34
Table 4. Surface area of samples for test of surface roughness under CO-H2-H2O
atmosphere ... 34
Table 5. Surface area of samples for test of surface roughness under C2H6 atmosphere
Table 6. Designation for experiments for the evaluation of time and temperature. ... 35
Table 7. Surface area of samples for test of time and temperature under C2H6
atmosphere ... 35
Table 8. Surface area of samples for cyclic test. ... 36
Table 9. Average of change in mass after pre-oxidation treatment. ... 58
Table 10. Change in mass per sample for different times and temperatures of exposure.
Table 11. Dimensions of samples for test of surface roughness under CO-H2-H2O
atmosphere ... 85
Table 12. Dimensions of samples for test of surface roughness under C2H6 atmosphere
Table 13. Dimensions of samples for test of influence of time and temperature under
C2H6 atmosphere ... 86
LIST OF ABBREVIATIONS
AFA Alumina-forming austenitic stainless steel alloy
SS Stainless Steel
HK, HP Heat-resistant chromia-forming alloys
I would first like to thank my advisor Dr. Benjamin Church for accepting me into his
research group. His continuous support since the beginning of the project and his
guidance helped me consistently to take the right path. By supporting my attendance at
various conferences, engaging me in new ideas, and demanding a high quality of work,
he made me not only a better student but also, with his example of teaching, working
and human being, made me a better person.
I would like to thank my committee members Dr. Hugo Lopez and Dr. Ronald Perez.
Thanks to Dr. Lopez for the knowledge gained through his class and for the interest on
my research. Thanks to Dr. Perez for his support during my Master’s studies.
I would also like to thank Jim Myers of MetalTek for providing his industrial insight, time
and resources throughout the project. Additionally, thanks to Dr. Steven Hardcastle for
his time and resources in the AAF, especially with the SEM and XRD trainings.
I would like to thank the research group members, Kao Yang, Elmer Prenzlow and
Wen-Chieh Lee, for their continuous help and friendship. Every result described in this
document was accomplished with their help and their support.
Finally, I must express my gratitude to my parents and to my host family, for providing
me with unfailing support and continuous encouragement through my Master’s Studies. This accomplishment would not have been possible without them.
This work was sponsored by ARPA-E, DE-AR0000690. Without their financial support
CHAPTER 1. INTRODUCTION
Applications such as power generation, chemical processing, fuel cells, and high
temperature heat exchangers are exposed to high temperature aggressive gaseous
environments which limit the life expectancy. Coking is the process of carbon deposition
from a gas phase that is encountered in many reforming, cracking and other high
temperature processes that can lead to carbon build up causing reduced process
efficiency as well as corrosive attack and degradation of the alloy.
The ethylene production process and other petrochemical processes can be improved
by developing materials that resist coking, retain long-term oxidation and corrosion
resistance, and yet remain economically favorable for implementation. Typical alloys
used in these applications are austenitic Fe-Ni-Cr heat resistance steels which form a
protective chromium oxide (chromia) layer during exposure. The chromia layer acts as a
diffusion barrier that restricts the transport of gas-phase constituents (oxygen, carbon)
and alloy constituents (Fe, Ni, Cr, and others) so that the inevitable reactions between
the gas and solid are slowed (1), (2). These heat resistant stainless steels rely on
chromia scales for protection from high temperature oxidation but their performance is
limited in many industrial environments. Depletion of chromium in the alloy due to
carburization can degrade the alloy’s ability to regenerate a protective oxide scale thus resulting in faster coke build-up and further carburization.
More recently, research into alloys which produce protective layers of aluminum oxide
(alumina) have been explored as a way to further slow the rates of high temperature
thought to be an alternative to the traditional alloys due to more stable oxide scale as
well as superior corrosion and creep resistance for many industrial environments (5).
The protective oxide layer enables the use of these alloys at higher temperatures and
for longer time periods than stainless steel alloys that form a protective chromium oxide
surface layer. This oxide layer make them suitable for a wide range of energy
production, chemical, and process industry applications, where the use of more durable
materials capable of withstanding higher temperatures can result in significant cost and
energy savings as well as reduction in environmental emissions (6). Development and
commercial implementation of such alloys is not trivial; a modification to chemical
composition alters the manufacturability of the material and long-term performance
remains an unproven, yet critical, variable.
Ethylene (C2H4), or ethene, is a hydrocarbon material used as a raw building block for
many industrially critical materials such as polyethylene, PVC, polystyrene, ethylene
glycol, and countless other products. The annual world-wide production is over 100
million tons with US production representing roughly 25% of the total. US based
production is expected to increase from an average of 1.25 million barrels per day (b/d)
in 2016 to 1.7 million b/d in 2018.1 Ethylene as one of the great buildings blocks in
chemistry is produced in large volumes mainly by thermal cracking of hydrocarbons in
the presence of steam, and by recovery from refinery cracked gas.
1 U.S. Energy Information Administration. “U.S. Gas Plant Production of Ethane-Ethylene”. www.eia.gov . Accessed
More than half of the production of ethylene is used to produce polyethylene, one of the
most important materials today. The market grows continuously with an average rate of
4% worldwide and can be related to the gross national product growth in an area or a
certain country (7).
The production of ethylene today is based on feedstocks derived from crude oil or from
natural or associated gas (Natural Gas). The leading technology applied for production
of ethylene is steam cracking, a high temperature pyrolysis in the presence of steam,
which was developed in the 1960s, and has remained largely unchanged since that time
(7). It is commonly produced in steam crackers where gaseous feed stocks such as
ethane or propane are cracked and formed into the ethylene structure. Hydrocarbons
and steam pass through tubes that are heated to temperatures above 900°C in many
cases exceeding 1100 °C. The systems for producing this raw chemical incorporate
large reactors that are made of alloys that provide 1) high temperature mechanical
strength and 2) chemical resistance to attack under the aggressive carbon-rich
conditions of the system. Typical alloys for the reactor tubes are stainless steels or
Fe-Cr-Ni centrifugal cast alloys (HK, HP). It is important to select the alloy composition or
control the environment to minimize the damage produced by interactions with
aggressive oxidants (8). Even with good alloys and tight process control, carbon
build-up (coking) is inevitable. Most production facilities are periodically taken off-line so that
the reactor system can be “de-coked” using steam and air to “burn off” coke deposits. The periodic maintenance results in a loss of production efficiency (~2-8% of annual
capacity), added costs, and thermal cycling of the system which imparts additional wear
1.2. Literature review
1.2.1. Current materials
Heat-resistant structural and related iron and iron-nickel alloys are used in corrosive
environments at temperatures above ~600 °C and up to ~1150 °C. These steels are
used in high temperatures environments that include air, ammonia, carburizing gases,
oxidizing and reducing flow gases. Such applications demand an optimum combination
of microstructural stability, creep resistance, excellent oxidation resistance, and
additionally, resistance to coking and carburization in case of ethylene pyrolysis
applications (9). These alloys utilize Cr2O3-based scales for protection. However, this
chromia scale can be susceptible to accelerated oxidation in the presence of water
vapor (10). The excellent metallurgical compatibility of chromium in Fe/Fe(Ni) allows
ready formation of a protective Cr2O3-based scale with wide alloy design flexibility
optimizing oxidation resistance with other needed properties such as creep resistance,
weldability, etc. (11). Because they combine good creep strength and oxidation
resistance, are widely used in energy production and chemical processing
environments. However, strong oxidation, carburization, sulfidation or nitriding can
occur if the environment does not promote chromium oxide formation or if the
protectivity of the scale is destroyed by other mechanisms (8).
1.2.2. AFA Alloys
Alumina-forming austenitic stainless steels have been recently developed for structural
use in aggressive oxidizing environments at 600-900 °C. These alloys show a promising
for good welding behavior. Recently investigations indicate the potential to achieve
superior oxidation resistance compared to conventional Cr2O3-forming iron- and nickel-
based heat-resistant alloys (11). This is due to the slower growth rate and greater
stability of alumina, particularly in the presence of water vapor species encountered in
many industrial process and energy production environments (12).
Studies shown these alloys have potential in process environments involving aggressive
water vapor, carbon, and sulfur species in temperatures ranging from 500 to 900°C. (6)
It is speculated that the key factor controlling if and how long Al2O3 scale formation
occurs in AFA alloys is oxygen solubility in the alloys. To promote protective Al2O3 scale
formation, it has been explored that alloying addition levels of ~4-6 wt.% aluminum and
~10-25 wt.% chromium can destabilize the parent austenitic matrix structure, resulting in
duplex ferritic/austenitic microstructure and a loss of creep resistance. This structure
can be stabilized by additions of nickel so the AFA alloys can develop a good oxide
scale and retain good creep resistance for the application (11) (see Figure 1 and Figure
188.8.131.52. Alloying additions
The alloy’s composition range have been studied so a material able to produce a good alumina oxide scale combined with a good creep resistance can be achieved.
Researchers have been developed different grades of AFA alloys and have been tested
in different oxidizing – carburizing environments at different high temperatures ranges (~600 - 1000 °C). Generally, the addition of Al and Cr to steel to increase its corrosion
investigations have been focused in the balance between Al, Cr and other alloying
elements so an optimal alloy can be developed.
Figure 1. Phase diagram of Fe-Cr-Al-(20, 25, 30) Ni-1Nb-2Mo-0.1C showing limitations of Cr and al additions in a range of 600 to 1200 °C (right); and at 650, 700, 750 and 800°C phases, predicted by
Figure 2. Superimposed ternary phase diagram of Fe-Cr-Ni near the Fe-rich corner at 1200 °C (bold lines) and at 800 °C (broken lines). Arrows indicate the direction of phase boundaries shifting by
the Al addition due to the strong δ-Fe stabilizing effect of Al relative to γ-Fe.2
2 Image taken from Yamamoto, Y. et al., “Overview of Strategies for High-Temperature Creep and
Studies on the alloy composition have explored the effects of alloying additions on
oxidation and creep behavior concluding:
It has been identified that AFA alloys with a relatively low Al and Cr contents (2.5 to 4 wt.% and 14 to 15 wt.% respectively, have formed alumina scale and permitted
stabilization of an FCC austenitic matrix phase for creep strength with low additions
of Ni (6).
Niobium additions (0.6 to 3 wt.% Nb) seems to enhance the oxidation resistance, particularly in water-vapor containing environments (6) (11).
Increasing niobium, aluminum, and/or nickel content all favor the establishment and maintenance of protective Al2O3 scale formation in these alloys (13).
Some tolerance for vanadium and titanium is important because they can be used to enhance MC carbide formation for improved creep resistance (11).
Use of nitrogen, titanium, and vanadium degrade the ability to form an alumina a surface layer in the AFA composition range and must be minimized (6).
Alloys can be strengthened by gamma prime precipitates (γ’-Ni3Al) with the proper balance of Al, Ni, Nb, and Ti additions (6).
Carbides precipitates should be incorporated for creep strength (6). C levels of 0.3 – 0.4 wt.% C are required to balance creep properties with oxidation resistance (11).
It has been found that cast AFA alloys containing 14wt.% Cr - 3.5 wt.% Al with approximately 25 wt.% Ni are restricted to maximum operating temperatures of
The creep resistance of the alloys seems to be strongly dependent on the level of Nb additions. Al additions also help to increase the creep resistance (14), (15).
1.2.3. Al2O3 vs. Cr2O3
Different types of low cost Fe- and Ni- based alloys are widely used to meet the
requirements of heat exchangers, steam crackers or tubes in the petrochemical
applications. However, because of higher operating temperature and aggressive
environment, most of the materials are not suitable for such applications. Above 700 °C,
the commonly used alloys are susceptible to severe oxidation and creep deformation.
The presence of water vapor (especially during the de-coking process), accelerates the
rate of oxidation and increases Cr evaporation. The stability and the performance of the
alloys are influenced by several factors such as microstructure, grain size, chemical
composition, phase precipitation, scale formation, and operating temperature (16).
Al2O3 scales offer a superior degree of protection to Cr2O3 scales in many
high-temperature environments (11), (17). Bhowmick et al. (16) studied the chromium
evaporation from chromia and alumina forming alloys at 850 and 950 °C for 500 hours
in air containing 2.6% and 12% water vapor. Chromium evaporation rate from thermally
grown alumina scales is approximately two orders of magnitude lower than that formed
on a conventional chromia forming alloy. They explained that the lower Cr evaporation
rate in the alumina-forming alloy is due to the development of thin protective alumina
scale on the surface along with the formation of Cr, Fe and Ni-rich islands.
A comparison of the advantages and disadvantages of the alumina scale versus
Table 1. Comparison of Al2O3 vs Cr2O3 oxide scales
Al2O3 scales grow at a rate that is 1 to 2
orders of magnitude lower than that of Cr2O3. (see Figure 3).
The presence of water vapor, accelerates the rate of oxidation and increases Cr evaporation
Diffusion of carbon (DC) is lower through
alumina than chromia.
Aluminum additions also reduce Dc within
Chromia (and spinel) prevent inward carbon diffusion under certain conditions by means of very low diffusion rate of carbon (Dc)
Alumina is more thermodynamically stable to higher temperatures and for longer time periods than chromia. (See Figure 3).
Loss of Cr through evaporation of Cr2O3
and/or CrO2(OH)2 at high oxygen partial
pressures >1850 °F (~1000 °C) which represents a temperature limitation.
Greater stability in the presence of water vapor (11). Significant oxidation volatility is not typically observed until temperatures reach ~1200 °C (6).
Volatile chromium oxy-hydroxide species can form and significantly reduce oxidation lifetime of the alloy (6).
A uniform and dense alumina scale can reduce the propensity for catalytic coke formation.
Local breakdowns in scale and subsequent transport of carbide or Fe ions to surface act as nucleation sites for catalytic coking.
It has been proven to be particularly beneficial in the presence of aggressive carbon- or sulfur-species encountered in combustion and chemical process industry applications (11), (17).
Above ~1900°F(1040°C) in the presence of carbon (i.e. coke layer), Cr carbide is thermodynamically favorable and its
formation will cause eventual failure of oxide layer
Figure 3. A schematic representation of (a) growth rate data and (b) thermodynamic stability data for specific oxides.
The arrows demark differences between Al2O3 and Cr2O3. 3
1.2.4. Crystal structure of AFA alloys
Ferritic Fe-Cr-Al-based alloys capable of forming Al2O3 are widely used in specialty
applications such as heating elements and furnace liners. However, they are not
suitable for structural applications above ~500-600°C because of its poor creep
resistance resulting from their open body-centered cubic structure. Investigations have
shown that to obtain a good creep resistance, an austenitic face-centered cubic
structure is needed.
Image taken from Brady, M. P. et al. “The development of alumina-forming austenitic stainless steels for high-temperature structural use”, 2008. (11)
Austenitic stainless steel has a face-centered cubic (FCC) crystal structure that is
stabilized by nickel; exhibits better high-temperature creep strength than ferritic
stainless steel, which features a body-centered cubic (BCC) crystal structure.
Studies in the role of Manganese in the high-temperature oxidation resistance of AFA
alloys have been done above 800 °C in air and in air with 10% water vapor. Manganese
is a strong face-centered cubic stabilizer and much cheaper than nickel, usually added
into austenitic steels to realize solid-solution strengthening, stabilize the austenite
matrix, and reduce the raw material cost. AFA alloys usually have between 1% and 2%
Mn, but its role in the oxidation process is not well clarified yet. Researchers have found
that excessive additions of Mn in AFA alloys tend to stimulate formation of the coarse
spinel CrMn1.5O4 and Cr2O3 which is responsible for the degradation in the oxidation
performance. Therefore, Xiangqi et al., have concluded that exists an upper limit for the
Mn addition, and the tolerable amount of Mn in these alloys is decreased with the
increase of the service temperatures and presence of water vapor. Also, they found the
oxidation resistance was moderately degraded with additions of larger than 1% Mn at
800 C, even in dry air (18).
The oxidation phenomenon is considerate as the most important corrosion reaction at
high temperature and is one of the primary considerations that determine the durability
of heat-resistant alloys. The metals and alloys oxidize when are exposed to air or
environments with high oxygen potential, at elevated temperature with a strong effect of
temperature over oxidation rate (17). The key factor for a good oxidation resistance is to
oxide phase (11). For high-temperature applications, such as higher than 600 °C, Cr2O3
and Al2O3 are the principal oxides used for the protection of metallic alloys.
Muralidharan et al., tested an AFA alloy (CAFA 7) cetrifugally cast in an oxidation
environment of air with 10 vol. % water vapor, and laboratory air (no added water
vapor). Oxidation exposures were conducted in 100 h cycles at 750 and 800 °C, and
800°C and 900 °C for 1000-2000 h using 500h cycles respectively. Their results show
that the oxidation resistance of the alumina forming stainless steels was superior to the
chromia-forming alloys (HK4 and HP5 steel). Figure 4 shows a BSE-SEM images of their
alloys after exposure to air for 2000 hours at 800 °C. It is noticeable that the oxide layer
formed by the AFA alloy is thinner than that formed by the HP alloy for the same
exposure conditions. They also report that in some regions of the AFA alloy, the oxide
layer was multi-layered, with the outside layer comprising of a locally nodular-like
Fe-Ni-Cr rich oxide, undercut by a continuous alumina layer. The oxide on HP was
multilayered in some regions as well, with the same nodular-like Fe-Ni-Cr rich oxide
followed by an interior layer being rich in Cr (9).
HK austenitic s.s.: 24-28 wt.% Cr, 18-22 wt.% Ni
Figure 4. BSE BSE-SEM image from CAFA7 (left) and HP (right) alloy tested at 800°C in air for 2000 hours.6
Since the formation of the alumina scale in the AFA alloys occurs at a slow growth rate,
the change in mass for the samples after exposure, even after 5000h have been
reported as a positive mass gains around <0.5 mg/cm2 (19). These small changes in
mass are consistent with protective alumina scale formation in the range of a few
microns thick (20). Researchers have found the scale to consist primarily of Al and O,
with only minor amounts of Cr, Fe, Mn, and Nb (21).
Yamamoto et al. tested AFA alloys (range composition of 20wt. % Ni – 12-14 wt.% Cr – 2.5-4 wt.% Al) for 1000 hours in air and in air with 10% water vapor environments at 650
and 800 °C finding that none of the current compositions formed protective alumina
scales at 1000 °C in air. However, excellent oxidation resistance at 650 and 700 °C was
observed. The loss of protective oxidation behavior was associated with a transition to
internal oxidation and nitridation of Al. Furthermore, the solubility of al in the austenitic
matrix is on the order of ~2 to 2.5 wt.% Al, so that the higher-Al containing alloys,
exhibited second phase dispersion of B2[(Ni,Fe)Al] (see Figure 5) acting as a Al
reservoirs for the growth of alumina scales (19).
Image taken from Muralidharan, G. et al. “Development of Cast Alumina-forming Austenitic Stainless Steel Alloys for use in High Temperature Process Environments”. (9)
Figure 5. BSE-SEM of AFA 4-1 (4Al/0.6Nb/0.1ti) after 100h at 900 °C in air.7
Thermodynamically, it is probable the formation of an oxide over a metal surface when
the oxygen potential in the atmosphere is higher than the partial pressure of oxygen in
equilibrium with the oxide. This partial pressure in equilibrium could be determined from
the standard free energy change (ΔG) for the oxide formation, considering this reaction:
Assuming the metal and oxide activities as the unity:
The standard free energy of formation for various oxides as a function of temperature
and the relative partial pressures of oxygen in equilibrium with the oxide are
summarized in Ellingham/Richardson diagram as shown in Figure 6. From this diagram,
it is possible to determine the potential of oxygen in oxidizing atmospheres (PO2) and
reducing atmospheres with gas mixtures (PCO/PCO2) (22). Comparing the oxygen
potential in the gaseous environment with the oxygen partial pressure in equilibrium with
the evaluated oxide, it is possible to determine thermodynamically if this is stable or not
under conditions worked in the laboratory.
Figure 6. Ellingham/Richardson diagram for metal oxides. Standard free energies of formation in function of Temperature.8
Millward et al. (23) used published algorithms to evaluate the free energy changes, ΔG, for the various oxidation reactions that can take place in the metal’s surface as show in Figure 7.
Figure 7. Free energy changes, ΔG, expressed as oxygen potential for various oxidation reaction
From Figure 7, it is appreciated that at temperatures of 850 – 915 °C, temperatures worked for the oxidation tests of this document, ratios of 102 -103 of H2/H2O are required
to form a Cr2O3 scale oxide on the surface of the metals.
9Image taken from Millward, G. R., Evans, H. E., Aindow, M., & Mowforth, C. W. (2001). “The Influence of Oxide Layers on the Initiation of Carbon Deposition on Stainless Steel” (23)
17 184.108.40.206. Kinetics
Church et al. (24), evaluated the relative oxide formation of a traditional chromia-forming
alloy (35Cr-45Ni-0.4) against two alumina forming alloys (27Cr-35Ni-0.4C) containing
varying amounts of aluminum (2.7%Al and 2.6%Al). The oxidation treatment was
intended to produce a stable surface oxide on the samples. Their environment
conditions were 850°C for 12 h and raised the temperature up to 915°C for 1, 10 and
100 hours in 100% steam. They concluded that the alumina forming alloys had
parabolic oxidation kinetics while the chromia forming alloy had significant departures
from parabolic behavior likely due to chromia volatilization. Furthermore, both
alumina-forming alloys were able to form a continuous layer during 100% steam oxidation. The
chromia-forming alloy showed mass changes that were non-linear with the root of time
indicating that is likely to had competing mechanisms of a) oxidation and b) chromia
Figure 8. Mass change of samples during steam pre-oxidation treatments at 915 °C.
Linear trend lines were forced to originate at the origin to emphasize ideal parabolic (Δm ∝ t0.5) kinetics.10
The formation of carbon deposits (coking) has been described in the literature and is a
function of several factors including the balance of hydrocarbon to steam, incorporation
of process gas dopants (e.g. sulfur compounds), and the surface chemistry of the
materials that make up the reactor (25), (26). Understanding the relation between the
alloy’s surface chemistry and coking resistance is a primary goal which will allow for the design of alloys with improved coking resistance.
The industrial environments normally connected to the metal dusting – problem contains CO, H2 and sometimes also other gaseous components, i.e. synthesis gas mixtures.
Image taken from Church, B., Ortiz, L., Prenzlow, E, et al. “An Initial Evaluation of the Effect of Alloy Composition and Oxide Layer on High Temperature Coking Resistance of Heat Resistant Alloys”, 2016 (24)
1.00 2 4 6 8 10 12 Spe ci fi c M ass Ch an ge (m g/ cm 2 )
Root time (h0.5
)Al-1 (3.7% Al) Al-2 (3.2% Al) 3545 MA
Basically, there are two reactions that bring about solid carbon or coke deposition in H2
Reaction (1.4) corresponds at Boudouard equilibrium and (1.5) to Steam-carbon
Szakálos et al. (5) investigated the kinetics of these reactions as a function of CO/H2
content and temperature on pure iron. The results showed that reaction (1.4) dominates
at higher CO concentrations and reaction (1.5) dominates at higher H2 concentrations
Thermodynamically, the carbon activity in the environment is determined according with
the present gaseous species like CO, CO2, H2O and H2, based on (1.4) and (1.5)
reactions. The, the carbon activity in the environment could be calculated from reaction
ΔG Gibbs energy change T Temperature of the system Pi Partial pressure
ac carbon activity in the gaseous environment
Considering the equilibrium constant of the reaction (1.5), then, it is possible to get an
The values of ac increase with decreasing temperature and may easily reach ac=100 or
1000 at low PH2O. The carbon from the reaction (1.5) may
a) be transferred into solid solution in the phase metal,
b) be consumed by carbide formation or
c) deposited as more or less graphitic carbon (27).
The thermodynamic condition to predict if an alloy would be carburized or decarburized
depends on the carbon activity (ac) in the environment and the interior of the alloy(28).
The alloy tends to be carburized or gain carbon from the environment when:
The alloy tends to be decarburized or lost carbon from the metal matrix when:
It may be concluded that during carbon deposition of high alloyed steels and Ni-base
alloys, two additional reactions take place which produce carbon from the gas phase
according to the reactions
It has been demonstrated that, metal dusting is caused by the strong tendency for
graphite formation, either by “graphitization” as in the case of nickel and Ni-base alloys or by carbide, mainly M3C decomposition as in the case of iron and steels (27).
Metal dusting has been also observed in refineries cause by naphtha and in principle
also in cracking tubes for ethylene production. Then, the carbon activity results from the
decomposition of hydrocarbons
If the environment contains CH4, the carbon activity of the environment will be
dominated by the reaction (1.13).
Where carbon activity can be expressed as
If the environment contains CO2/CO/C2H4 gas mixture, the carbon activity of the
CO2/CO equilibrium will be negligible compared with that produced by the reaction of
ethylene (C2H4) with other constituents. Various possible overall dissociation reactions
can be identified (23):
The carbon activity of this environment is uncertain, since it depends on which of the
reactions (1.15), (1.16), or (1.17) will dominate and how closely equilibrium is
approached. Even so, carbon activities far greater than unity can be expected and that
the gas, will provide a potentially highly depositing environment.
Serna et al. (8) report that boundary grain precipitation is the main mechanism of
carburization in austenitic Fe-Ni-Cr (HP-40) alloys was observed for samples extracted
from ethylene furnace tubes. They saw internal carburization only in areas where the
oxide film was absent. For austenite, carbon solubility is high, but carbon diffusivity is
low, and chromium diffusivity is low. For ferrite, carbon solubility is much less but carbon
diffusivity is much higher; chromium diffusivity is much higher.
In general, three coke formation mechanisms have been described in the literature: the
heterogeneous catalytic mechanism, the heterogeneous free-radical mechanism, and
the homogeneous droplets condensation/tar deposition mechanism (29).
The catalytic mechanism, accounts for the coil materials, with nickel and iron acting as
catalysts for the formation of carbonaceous deposits in carbon-rich atmospheres. In this
mechanism, as shown in Figure 9, hydrocarbons are chemisorbed on the metal surface,
subsequently losing hydrogen atoms which react and desorb into the gas phase. The
carbons left at the surface start diffusing into the alloy. As carbon keeps depositing, the
particles keep being lifted by carbon filaments growing out of the surface.
eventually covers the particle, encapsulating it. Therefore, the relative importance of
radical coking compared to that of catalytic coking increases over time (29).
Figure 9. Schematic diagram of the heterogeneous catalytic mechanisms for coke deposition.11
Respect to the heterogeneous free-radical mechanism can be explained by five radical
reactions: hydrogen abstraction, substitution, addition by gas phase radicals, addition to
gas phase olefins and cyclization. This radical mechanism is present throughout the
entire run length of the coil, and its relative importance increases over time as the
catalytic sites of the surface are covered (29).
The homogeneous droplet condensation mechanism applies when heavy polynuclear
aromatics are present in the atmosphere. Its importance relies when cracking heavier
feeds, such as gas oils, vacuum residue, and bitumen are cooled (29).
11 Image taken from Andres Munoz et al., “Influence of the Reactor Material Composition on Coke
Kinetics of coke formation have been studied in some alloys in atmospheres similar to
petrochemical industry atmospheres. Jackson et al., studied the coking kinetics of
several commercial Fe-Ni-Cr alloys used as materials for ethylene steam crackers.
Temperatures of 450 to 1000°C in hydrogen-propylene atmosphere using a
microbalance reactor were used. They found that the rate of coke formation on alloys
increased continuously between 500 and 1000 °C. Between 900 and 1000°C, steady
state kinetics were controlled by gas-phase pyrolysis and similar reaction rates were
observed for all materials. Also, they conclude that differing catalytic activities resulted
in significant differences in coking rates below 900 °C; whereas significant differences in
reaction rates of alloys due to formation of filamentous coke was observed only below
Munoz et al. (29), studied the influence of the reactor material composition on coke
formation during ethane steam cracking, finding that coke deposition is strongly affected
by the composition of the material. Also, that Al-enhanced alloys had a better resistance
to coke formation than those without aluminum in their formulation. In general, they
conclude that for all alloys, independent on composition, the formation of a uniform layer
of a protective oxide is essential, because the stability of the surface after pre-oxidation
or decoking has a significant impact on the coking rate and not the bulk composition.
220.127.116.11. Composition and morphology of coke
Depending on the composition of the alloy and gas mixture, the coke will grow as a fur
uniformly on the samples, locally and/or in form of noodles, cones or leeches. On high
alloy steels the metal dusting and coke growth start locally in most cases, at spots
carried away by the gas flow and deposited somewhere in corners or dead ends.
Chemical analysis can prove if the coke is from metal dusting, where will always contain
metal elements. The metal components of the corroding alloys are transferred into the
coke always in ratios corresponding to the alloy composition as carbides or oxides.
Then, the morphology of coke can be very different depending on the steel, its surface
state, the reaction temperature, and other parameters (27).
18.104.22.168. Metal dusting – CO/H2/H2O gas atmospheres
Metal dusting is a corrosion phenomenon that deteriorates iron, low and high alloy
steels, and other materials in strongly carburizing gas atmospheres, with carbon activity
ac>1 and at higher temperatures (usually 400-800°C). It is also defined as the
disintegration of alloys into carbon and metal particles during high-temperature
exposure to carbon-bearing gases (2). Corrosion products are graphite, metal, carbide,
and oxide particles, mixed in finely divided form. Depending on the composition of the
alloys and environment conditions, different mechanisms of metal dusting have been
described in the literature.
J. Zhang et al. (31) characterized the coke formed by carburizing a pure iron sample at
700°C in a 24.81 – 94.81 vol.% H2, 5-75 vol.% CO and 0.19 vol.% H2O gas mixture covering a range of carbon activities (15.8 ≤ ac ≤ 82.9). They found the carburization is fast at the early stage of the reaction, then this rate decreases slightly and finally
increases drastically after 2-hour reaction. Formation of a cementite with a graphite
layer was found on the surface of the cross sections of the samples. Also, after 4 hours
of carburization, a thick coke layer was found on the surface. They conclude that nature
(ac=15.8), a major part of α-Fe particles together with cementite and some Fe2C can be found on the surface. If the CO content exceeds 30% only iron carbide is observed in
the coke for a test with pure iron samples.
Toh et. al (2) studied Fe-Cr and Fe-Ni-Cr alloys under 68%CO-26%H2-6%H2O gas
mixtures at 680 °C (ac = 2.9) under thermal cycling conditions. They assumed that
interstitial diffusion of carbon into the alloy is much faster than substitutional diffusion
and the process is one of carbon enrichment in a system in which the Fe/Cr ratio
remains fixed. Depending on the composition of the alloy and the Fe/Cr ratio, a diffusion
path may be followed in the ternary diagram of the Fe-Cr-C system.
Based on Figure 10, the corresponding diffusion path for an Fe-46Cr alloy is shown.
This composition is critical since at lower chromium levels, the formation of Fe3C is
predicted whereas at higher levels it is not. Then, alloys containing more than 46% Cr
would be predicted to resist dusting. However, additions of Ni to the Fe-Cr-C system
results in destabilization of both ferrite and Fe3C. At nickel levels of 10 and 25%, the
Fe3C phase is completely suppressed and only the chromium-rich carbides are
predicted to form under the conditions of the test. They concluded that loss of
chromia-reheating ability was followed by spinel formation, internal carburization, and surface
cementite formation was found on the alloys after being tested. The difference in the
nature of the “metal-dust” particles was reflected in the coke morphology and corresponded to large differences in metal-wastage rates (2).
Figure 10. Isothermal ternary diagram for Fe-Cr-C system at 680 °C.
Dashed line shows a possible diffusion path for Dc>>Dm for a Fe-46Cr alloy 12
22.214.171.124. Hydrocarbons atmospheres
In the refinery and petrochemical industries, austenitic and ferritic alloys are usually
used for tubes in fired furnaces where environments are combustion product gases and
hydrocarbon gases with low oxygen potentials and high carbon potentials. Usually, the
temperature range for exposure of austenitic alloys is 800-1100 °C, and for ferritic alloys
500-700 °C. These processes involve carbon deposition (coking) on the inner diameter,
carbon absorption at the metal surface, diffusion of carbon inside the alloy, and
precipitation and transformation of carbides to a depth increasing with service (8).
During thermal and steam cracking operation, carbon is deposited in the form of coke
on the internal surfaces of the tubes. The efficiency of heat transfer is reduced and the
12 Image taken from “Metal Dusting of Fe – Cr and Fe – Ni – Cr Alloys under Cyclic Conditions. Oxidation
metal skin temperature increased to maintain the process temperature. The presence of
coke eventually leads to carburization of the tubes when it is periodically removed by
oxidation in water vapor and air (de-coking) (8).
Serna et al. (8) compared the morphological differences in the carbon deposition
occurred in austenitic and ferritic alloys exposed for a long time in environments with
carbon activity over one in many cases concluding:
In a sample of a ferritic alloy Fe-9Cr-1Mo extracted from a tube closed to the outlet of the radiation zone, exposed for 102000 hours at 600 °C showed the evident bulk
carburization through all the cross section along the inside diameter. Although this
alloy had an oxide layer over the internal surface, the carburization was
homogeneous along the internal diameter.
A tube alloy of austenitic Fe-Ni-Cr (HP40) extracted from a coil of the radiation zone of the furnace exposed for 88000 hours over 900 °C, carburization only occurred
along the austenitic grain boundary. A pre-existing oxide scale over the internal
surface in this alloy, formed in air before exposure to the carburization environment,
reduced or inhibited carburization. Internal carburization was present only in areas
where the oxide film was absent.
Investigations of carbon deposition on stainless steels have been done as well. Millward
et al. (23) studied the influence of oxide layers on the initiation of carbon deposition on
stainless steels. With a 102 < ac < 107, they tested two 20Cr-25Ni-Nb-stabilized
austenitic steels containing either zero or 0.56 wt.% Si using CO2/CO/C2H4 gas mixture
at 550 °C. Their research confirmed that carbon filaments are not readily nucleated on
versions of the alloy, neither chromia nor magnetite catalyzed carbon deposition under
those test conditions. However, carbon deposits may have formed in regions covered
by iron-rich oxides provided there is gas access to catalytic sites within the alloy
substrate. They have postulated that these are regions of metallic nickel formed (see
Figure 11) as a result of the selective oxidation of chromium and iron by the depositing
Figure 11. Schematic depth profile illustrating a suggested mode of formation of nanoparticles of Ni that can act as potential catalytic agents for producing carbon filaments13.
1.2.7. Cyclic conditions
Investigations on HP40Nb alloys previously preoxidized and subsequently exposed to
an alternating carburizing/oxidizing/carburizing atmosphere at 1000°C have concluded
that a thick Cr2O3 layer formed on surface which partly spalled off during cooling to
room temperature, in this way chromium depleted areas resulted at the surface (32).
Additionally, during second exposures to the carburizing atmosphere there is more
catalytic coke formation compared to the first exposure showing that, the reduction of
the oxides promotes the formation of (Fe, Ni)-particles which show strong catalytic
activity towards coke formation (30).
13 Image taken from “The Influence of Oxide Layers on the Initiation of Carbon Deposition on Stainless
The catalytic coke formation during thermal cracking in hydrogen rich hydrocarbon
atmospheres is cause by the presence of a porous (Fe, Ni, Cr-) spinel layer at the metal
surface which is formed during the oxidation step. However, severe pre-oxidation of the
metallic surface followed by rapid cooling and spalling of the oxide layer causes
chromium depletion. Once there is chromium depletion and there is contact with a
carburizing atmosphere, formation of rich carbide decreasing the chromium
concentration of the metallic matrix. Finally, repeated coking operations result in the
reduction of the spinels into highly catalytic Fe and Ni particles leading to grow a
CHAPTER 2. METHODOLOGY
An experimental high temperature coking atmosphere was constructed and used to
evaluate the effects of temperature, time and metal surface roughness on the carbon
deposition of two alumina forming alloys. Furthermore, the same alloys were evaluated
in one coking/de-coking cycle to compare early-stage performance and identify if oxide
spallation would be observed. Coking conditions were simulated with multiple
atmospheres including CO-H2 mixtures at moderate temperatures and ethane at higher
temperatures. Carbon deposition was tracked using specific mass change of the
samples as a function of exposure times and conditions. Results obtained with the
alumina forming alloys were compared to a baseline HP alloy. The materials were
characterized using SEM and EDS to characterize the oxide layer formation, carbon
deposition layers and carbon attack, and changes to base metal microstructure. Raman
spectroscopy was used to characterize the carbon deposits.
2.1. Material Composition
A series of alloys were produced via centrifugal casting process and provided by
MetalTek International, were received as sections of pipe. The production process used
is identical to that used to produce production tubes for ethylene service. Following
horizontal centrifugal casting, the cast tubes were pull-bored to machine the inner
diameter. The inner diameters of the tubes were pull bored and the outer diameter was
left in the as-cast condition. Three alloys were chosen for the experiments. The nominal
alloy compositions are shown in Table 2. Two AFA alloys against one chromia forming
are being tested. The difference between AFA alloys is the Aluminum compositions
relatively similar. The chromia former alloys does not have aluminum and its Cr-Fe and
Ni-Fe ratios are similar to the AFA alloys.
Table 2. Nominal compositions of the alloy samples.
Nominal Composition wt%
Designation Fe Al Cr Ni Nb Si Mn C MA additions
H 3.7 % Al Remainder 3.7 27 34 0.8 1.3 0.6 0.4 Ti, Zr added
L 2.6 % Al Remainder 2.6 28 38 0.7 1.3 0.8 0.4 Ti, Zr added
C HP-Nb Remainder 0 27 34 0.8 1.3 0.6 0.4 Ti, Zr added
Both 3.7% Al and 2.6% Al are designed as alumina-forming austenitic alloys (AFA).
The HP-Nb is a Chromia forming heat resisting alloy. For easy handling of the samples,
“C” refers to the chromia forming, “H” to the 3.7% Al and “L” to the 2.6% Al AFA alloys. Change in mass was tracked during all steps of the experiments.
2.2. Sample preparation
Samples were prepared from as-cast pipe sections, cut down with an abrasive saw to
pieces of roughly the same dimensions (see Figure 13). Variables “x’ and “y” represent the inner and outer diameters; “t” the thickness of the samples and “h” the height. Following this, samples were ground to 600-grit in all sides of the cut surfaces, and
Figure 12. Notation for dimensions of samples after cutting
Figure 13. Some of the samples used for tests.
Prior to any test, samples were subjected to measurements. Each sample was
assumed to take the generic shape of a trapezoidal prism as shown in Figure 12.
Samples were ground until all sides were flat until there was no curvature from ID or OD
sides. Surface area of each samples was calculated using equation (2.1).
Where SA denotes surface area; “t” is thickness, “x” and “y” are the horizontal measurements and “h” is the height of the sample, all depicted in Figure 12.
34 2.2.1. Influence of surface roughness
The surface roughness that the material will have depends on the grit paper used. The
experiment used three different sandpapers to generate different surface finish on the
samples. These are shown in Table 3.
Table 3. Surface roughness average for each grit sandpaper used.
Std. ANSI Grit
Grit Median Diameter (micron) Surface roughness Ra (micron) 80 180 1.14 320 40.5 0.23 1200 2.5 0.02
Different samples were cut from the cast tubes, ground to 80-, 320- and 1200-grit on the
surfaces, and cleaned in methanol followed by acetone. Samples were averaged 7.35
cm2 for the CO-H2-H2O atmosphere and 7.90 cm2 for the C2H6 atmosphere test as
shown in Table 4 and Table 5. Specific dimensions for each sample can be found in
APPENDIX A – DIMENSIONS OF SAMPLES.
Table 4. Surface area of samples for test of surface roughness under CO-H2-H2O atmosphere
Surface area (cm2) Surface roughness 80 320 1200 Al - 3.7% 6.67 7.57 9.47 Al - 2.6% 6.72 7.87 6.82 HP - Nb 7.86 6.63 6.55
Table 5. Surface area of samples for test of surface roughness under C2H6 atmosphere
Surface area (cm2)
Sample Surface roughness
80 320 1200
Al - 3.7% 8.90 8.41 7.57
Al - 2.6% 7.05 7.28 6.76
2.2.2. Influence of time and temperature under C2H6 atmosphere
Experiments at 850, 950 and 1050 °C were performed for 1, 6 and 24 hours each. The
two AFA alloys were tested against the chromia-forming alloy under these conditions.
Samples were ground to 320- grit SiC paper. Under these conditions, nine experiments
were performed and the designation for the samples for each experiment are shown in
Table 6. Designation for experiments for the evaluation of time and temperature.
Time 850 950 1050
1 C1 H1 L1 C4 H4 L4 C7 H7 L7
6 C2 H2 L2 C5 H5 L5 C8 H8 L8
24 C3 H3 L3 C6 H6 L6 C9 H9 L9
Samples were averaged 6.99 cm2 in surface roughness for the C2H6 atmosphere test as
shown in Table 7. Specific dimensions for each sample can be found in APPENDIX A – DIMENSIONS OF SAMPLES.
Table 7. Surface area of samples for test of time and temperature under C2H6 atmosphere Surface roughness (cm2) Time Temperature 850 950 1050 1 6.72 7.28 6.54 7.59 7.37 7.31 7.42 6.23 7.88 6 5.95 7.53 6.73 6.29 7.36 6.84 6.71 8.05 6.89 24 6.41 7.85 6.22 7.16 7.12 6.13 6.79 6.51 7.88
36 2.2.3. Cyclic conditions
Samples were ground to 320-grit on the surfaces, and cleaned in methanol followed by
acetone. Experiments of pre-oxidation, coking, de-coking with air and de-coking with
steam were performed. Surface area of samples were averaged 6.80 cm2 as shown in
Table 8. Specific dimensions for each sample can be found in APPENDIX A – DIMENSIONS OF SAMPLES.
Table 8. Surface area of samples for cyclic test.
Surface area (cm2)
1 2 3 4
Pre-oxidation Coking de-coking
air de-coking steam HP-Nb 6.96 7.44 7.09 7.68 3.7 % Al 6.13 7.71 6.28 7.05 2.6 % Al 6.65 6.52 6.26 5.81
“1” denotes samples that will go until pre-oxidation; “2” coking; “3” coking with air; and “4” until de-coking with steam step.
2.3. Pre-Oxidation test
The purpose of the pre-oxidation procedure was to develop a known and controlled
distribution of oxide on the specimen surface prior to coking test. The apparatus is
designed so that temperatures of up to 1000 °C can be achieved in the furnace, while
steam is constantly flowed throughout the chamber. The process to obtain an
environment of pure steam includes the purging of the system with nitrogen prior to
switching to steam flow. It was used a small exchange furnace to produce steam
allowing only steam vent through the chamber while the flow rate of steam is held at
Figure 14. Oxidation Apparatus
Features of the testing setup (see Figure 14) are:
1. Peristaltic pump
2. Furnace for steam generation
3. Heating/Temperature controllers
4. Steam overflow vent during nitrogen use
5. Three-way heated inlet valve for nitrogen/steam change and three-way valve for
steam to furnace/atmosphere
6. Tube furnace with quartz 1” tube, and programmable temperature controller 7. Heated steam exit vent
Steam pre-oxidation was carried out using 100% steam environment as described in
Figure 15, running for 12 hours at 850°C followed by raising the temperature up to 915